Download presentation

Presentation is loading. Please wait.

Published byAmya Lippitt Modified over 2 years ago

1
1 Harvey N. Rutt, Suresh Uppal Chong Yew Lee Optoelectronics Research Center University of Southampton,Southampton SO17 1BJ Design of an Electrically Operated mid-infrared solid-state modulator AITA 7 th September 2005

2
2 Outline Background Choice of Material The physics Electrical modulator Design criteria Simulation results Outlook

3
3 The need for a modulator Built in calibration, ‘thermal referencing’ Variable IR transmission in situations where mechanical solutions are undesirable Image from pyroelectric detectors requires modulation IR Spatial Light Modulators?

4
4 Desiderata! –Polarisation insensitive –Copes with low F number beams, to F#1 –High on state transmission (>95%) –Low power consumption –High off state attenuation –Large aperture (to 1cm 2 ) –Full 8-14μm band –Fast – but slow OK for many applications. Difficult to satisfy simultaneously!

5
5 For a semiconductor, carrier based device we need: A stronger absorption mechanism than the free-carrier Drude-Zener A way to maintain large carrier densities at low power cost Hence a long lifetime Infrared transparency Availability!

6
6 Choice of Material Why Ge –Indirect bandgap – long intrinsic lifetime –IR transparent 1.8—18 um –Available in high purity (use in Nuc. Det.) –High carrier mobility –Availability + cost + ease of fabrication –p-type Ge has lh-hh interband transitions in required spectral range

7
7 The principle Band diagram of Ge showing heavy and light hole band

8
8 Absorption spectra Absorption spectra of intrinsic and p type Ge i

9
9 Optical modulator

10
10 Optical Modulator in action Off state ON state

11
11 Basic structure Optimise: Doping levels Width of p, i, and n regions etc Processing Note: The IR has to traverse The doped regions.

12
12 Design Criteria OPTICAL ON state (diode electrically off) T on =T o exp(-A) = T 0 exp -(N p *x p *σ h ) OPTICAL OFF state (diode electrically on) T off =T o exp(-A) = T 0 exp (n p *σ h ) [n p = 0 ∫ t c p (x)dx] Where T o =1 for 100% transmission A is the absorption σ h is hole absorption cross-section (5.33x10 -16 cm 2 ) N p is the doping density for holes (/cm 3 ) n p is the area carrier density when forward biased (p+i region) x p is the thickness of the p layer

13
13 Design Criteria ON state: max T on minimum N p *x p OFF state: min T off maximum n p Uniform current injection requires high doping density (N p ) ABSORPTION vs UNIFORMITY trade-off!

14
14 Lifetime requirement We had σ h =5.33x10 -16 cm 2 And T off =T 0 exp (n p * σ h ) [n p = 0 ∫ t c p (x)dx] Lets assume a uniform hole density And a 1mm thick device And require T off =0.01 (ie, 1%) Then we need n p =8.64*10 15 /cm 2 Or N p =8.64*10 16 /cm 3

15
15 Design Criteria: required lifetime Rough analytical estimates: OFF state (i layer) : n p =Τ a *J/q (T a =T p +T n )

16
16 Design Criteria: Doping (N p *x p ) ON state: 95% transmission requires an area doping density of ~1x10 14 /cm 2

17
17 P N i -V, Cathode +V, Anode Device Centre Voltage drop due to sideways current flow Lateral Current Flow Problem Very little injection occurs near the centre The problem also occurs on the N side, but is less severe

18
18 Carrier Mobility in Ge We require high mobility for uniform current distribution! Carrier-carrier scattering degrades mobility above ~ 1e15 /cm3 10 14 10 19 Doping concentration (cm -3 ) Mobility (cm 2 /Vs)

19
19 Drive voltage issues – intrinsic layer thickness 2d < La Carrier recombination in doped region, J decreases 2d > La Large drop across i region, Increased heat dissipation

20
20 Simulations: ‘standard’ Ge 10μS lifetime, typical of ‘standard’ material 10 18 /cm 3 acceptors P side, 10 14 /cm 2 5*10 18 /cm 3 donors N side, 5*10 14 /cm 2 Gaussian profile Axisymmetric 50μm wide metal ring electrodes

21
21 Hole concentration at 0.6 Volts REMINDER! We needed ~ N p =8.64*10 16 /cm3 Oh dear……..

22
22

23
23

24
24

25
25 Avoid Copper! Copper has an EXTREMELY high SRH cross section! Copper diffuses very rapidly through germanium Tiny concentrations, ~10 10 /cm3, severely shorten the lifetime. Nuclear Detector is satisfactory, with lifetimes ~5mS So we assume 2.5mS, allowing some processing loss Avoidance of copper contamination is CRUCIAL

26
26 Hole concentration at 0.4 Volts REMINDER! We needed ~ N p =8.64*10 16 /cm3 Hopeful…….

27
27 Hole concentration at 0.5 Volts REMINDER! We needed ~ N p =8.64*10 16 /cm3 Interesting……….

28
28 Hole concentration at 0.6 Volts REMINDER! We needed ~ N p =8.64*10 16 /cm3 Whoopeeeeee…..

29
29

30
30

31
31

32
32 BUT… There are issues…as always –Surface Recombination Velocity –Auger Recombination –Shockley-Read-Hall (SRH) Recombination –Photon transitions (indirect band gap) –Impact ionisation (high E.Field only) –Tunneling (not possible) –Many-body effects on diffusivity

33
33 What is Surface Recombination? For Ge S=1-100cm/s Conduction band Valence band Carriers diffuse to the surface And ‘kill’ the effective lifetime.

34
34 What is SRH Recombination Trap could be due to presence of foreign atoms such as Cu, Ni, Au or a structural defect in crystal The ultra-pure material is essential free of this But the heavily doped regions are damaged….

35
35 Concentration Dependent SRH No literature available on CONSRH in Ge, pure guess values!! Quite Pessimistic values assumed, a factor of 1/10,000 i.e. from 10mS to 1 uS at highest concentration! The effect only operates over a very small volume of the device

36
36 What is Auger Recombination? Three particle effect γ 3 =1.1e-31 cm 6 /s Some theoretical estimates lower (better) But not that well established at densities relevant to us.

37
37 Conclusions Some device modeling still needed for optimization Process simulation now more important Alloyed contacts may be used for fabrication? Lifetime preservation in processing absolutely crucial The Auger parameter is a concern But it does look possible

Similar presentations

Presentation is loading. Please wait....

OK

Author: Julia Richards and R. Scott Hawley

Author: Julia Richards and R. Scott Hawley

© 2017 SlidePlayer.com Inc.

All rights reserved.

Ads by Google